# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ines39
_database_code_depnum_ccdc_archive 'CCDC 1045308'
_audit_update_record             
;
2015-01-23 deposited with the CCDC.
2015-04-22 downloaded from the CCDC.
;

_audit_creation_date             2014-11-06T00:26:19-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'

#----------------------------------------------------------------------------#
#                   CHEMICAL INFORMATION                                     #
#----------------------------------------------------------------------------#

_chemical_name_systematic        'K0.13 Mg Mo3 Na3.87 O12'
_chemical_formula_sum            'K0.13 Mg Mo3 Na3.87 O12'
_chemical_formula_weight         598.18

#----------------------------------------------------------------------------#
#                   UNIT CELL INFORMATION                                    #
#----------------------------------------------------------------------------#

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   12.9325(8)
_cell_length_b                   13.5537(9)
_cell_length_c                   7.1627(6)
_cell_angle_alpha                90
_cell_angle_beta                 112.212(9)
_cell_angle_gamma                90
_cell_volume                     1162.33(14)
_cell_formula_units_Z            4
_cell_measurement_temperature    298(2)

#----------------------------------------------------------------------------#
#                   CRYSTAL INFORMATION                                      #
#----------------------------------------------------------------------------#

_exptl_crystal_density_diffrn    3.418
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1116
_exptl_special_details           
;
 ?
;

#----------------------------------------------------------------------------#
#                   ABSORPTION CORRECTION                                    #
#----------------------------------------------------------------------------#

_exptl_absorpt_coefficient_mu    3.49
_exptl_absorpt_correction_type   none

#----------------------------------------------------------------------------#
#                   DATA COLLECTION                                          #
#----------------------------------------------------------------------------#

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_monochromator  graphite
_diffrn_reflns_av_R_equivalents  0.0272
_diffrn_reflns_av_unetI/netI     0.0256
_diffrn_reflns_number            2712
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -1
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         2.27
_diffrn_reflns_theta_max         26.97
_diffrn_reflns_theta_full        26.97
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_reflns_number_total             1261
_reflns_number_gt                1220
_reflns_threshold_expression     >2sigma(I)

#----------------------------------------------------------------------------#
#                   COMPUTER PROGRAMS USED                                   #
#----------------------------------------------------------------------------#

_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'

#----------------------------------------------------------------------------#
#                   REFINEMENT INFORMATION                                   #
#----------------------------------------------------------------------------#

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0132P)²+7.1077P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_number_reflns         1261
_refine_ls_number_parameters     96
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0256
_refine_ls_R_factor_gt           0.0241
_refine_ls_wR_factor_ref         0.0584
_refine_ls_wR_factor_gt          0.0579
_refine_ls_goodness_of_fit_ref   1.229
_refine_ls_restrained_S_all      1.228
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_diff_density_max         0.811
_refine_diff_density_min         -0.657
_refine_diff_density_rms         0.12

#----------------------------------------------------------------------------#
#                   ATOMIC TYPES, COORDINATES AND THERMAL PARAMETERS         #
#----------------------------------------------------------------------------#

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0 0.21604(3) 0.75 0.01849(13) Uani 1 2 d S . .
Mo2 Mo 0.23694(3) 0.60958(2) 0.12685(5) 0.02006(11) Uani 1 1 d . . .
Mg1 Mg 0.21624(11) 0.34005(10) 0.12690(19) 0.0161(3) Uani 0.5 1 d P . .
Na1 Na 0.21624(11) 0.34005(10) 0.12690(19) 0.0161(3) Uani 0.5 1 d P . .
Na2 Na 0 0.23648(18) 0.25 0.0250(5) Uani 1 2 d S . .
Na3 Na 0.5 0.5 0.5 0.0412(7) Uani 1 2 d S . .
Na4 Na 0 0.4915(2) 0.75 0.0440(11) Uani 0.869(19) 2 d SP . .
K1 K 0 0.4915(2) 0.75 0.0440(11) Uani 0.131(19) 2 d SP . .
O1 O 0.6702(3) 0.0051(3) 0.6099(5) 0.0434(9) Uani 1 1 d . . .
O2 O 0.3951(3) 0.3654(2) 0.2540(5) 0.0387(8) Uani 1 1 d . . .
O3 O 0.3789(3) 0.5894(2) 0.1839(5) 0.0306(7) Uani 1 1 d . . .
O4 O 0.4566(3) 0.7902(2) 0.5302(4) 0.0265(6) Uani 1 1 d . . .
O5 O 0.3261(3) 0.8305(2) 0.1080(4) 0.0314(7) Uani 1 1 d . . .
O6 O 0.2769(3) 0.8203(3) 0.6735(4) 0.0326(7) Uani 1 1 d . . .



#----------------------------------------------------------------------------#
#                   MOLECULAR GEOMETRY                                       #
#----------------------------------------------------------------------------#

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O2 1.758(3) 8_456 ?
Mo1 O2 1.758(3) 7_556 ?
Mo1 O4 1.771(3) 4_546 ?
Mo1 O4 1.771(3) 3_445 ?
Mo1 Na3 3.4323(4) 3_445 ?
Mo1 Na3 3.4323(4) 4_546 ?
Mo1 Na1 3.4965(14) 1_556 ?
Mo1 Na1 3.4965(14) 2 ?
Mo1 Na1 3.5180(14) 8_456 ?
Mo1 Na1 3.5180(14) 7_556 ?
Mo1 Na2 3.5920(4) 1_556 ?
Mo1 Na2 3.5920(3) . ?
Mo2 O3 1.745(3) . ?
Mo2 O1 1.759(3) 8_455 ?
Mo2 O5 1.765(3) 7_565 ?
Mo2 O6 1.781(3) 7_566 ?
Mo2 Na1 3.5253(14) 4 ?
Mo2 Na1 3.5548(14) 6_565 ?
Mo2 Na4 3.6035(14) 1_554 ?
Mo2 K1 3.6035(14) 1_554 ?
Mo2 Na2 3.6113(12) 3 ?
Mo2 K1 3.7531(12) 5_566 ?
Mg1 O2 2.169(4) . ?
Mg1 O5 2.170(3) 4_545 ?
Mg1 O1 2.173(4) 8_455 ?
Mg1 O4 2.195(3) 4_545 ?
Mg1 O6 2.203(3) 4_545 ?
Mg1 O6 2.292(4) 6_565 ?
Mg1 Na1 3.350(3) 7 ?
Mg1 Mg1 3.350(3) 7 ?
Mg1 Na2 3.5260(17) . ?
Mg1 Na4 3.689(2) 1_554 ?
Mg1 K1 3.689(2) 1_554 ?
Mg1 Na4 3.960(2) 5_566 ?
Na2 O4 2.393(3) 3_445 ?
Na2 O4 2.393(3) 4_545 ?
Na2 O5 2.447(3) 4_545 ?
Na2 O5 2.447(3) 3_445 ?
Na2 O3 2.468(4) 3_445 ?
Na2 O3 2.468(4) 4_545 ?
Na2 Na1 3.5260(17) 2 ?
Na2 Mg1 3.5260(17) 2 ?
Na2 Mo1 3.5920(4) 1_554 ?
Na3 O3 2.523(3) 5_666 ?
Na3 O3 2.523(3) . ?
Na3 O2 2.543(3) 5_666 ?
Na3 O2 2.543(3) . ?
Na3 O3 2.686(3) 6_566 ?
Na3 O3 2.686(3) 2_655 ?
Na3 Mo1 3.4323(4) 3 ?
Na3 Mo1 3.4323(4) 7_556 ?
Na3 Na3 3.5813(3) 2_656 ?
Na3 Na3 3.5814(3) 2_655 ?
Na3 Na2 3.671(2) 3 ?
Na3 Na2 3.671(2) 7_556 ?
Na4 O1 2.684(4) 8_456 ?
Na4 O1 2.684(4) 7_556 ?
Na4 O1 2.749(4) 4_556 ?
Na4 O1 2.749(4) 3_455 ?
Na4 K1 3.5888(5) 5_567 ?
Na4 Na4 3.5888(5) 5_567 ?
Na4 K1 3.5888(5) 5_566 ?
Na4 Na4 3.5888(5) 5_566 ?
Na4 Mo2 3.6035(14) 1_556 ?
Na4 Mo2 3.6035(14) 2 ?
Na4 Na2 3.688(4) 5_566 ?
Na4 Na1 3.689(2) 2 ?
O1 Mo2 1.759(3) 8_556 ?
O1 Na1 2.173(4) 8_556 ?
O1 Mg1 2.173(4) 8_556 ?
O1 K1 2.684(4) 7_556 ?
O1 Na4 2.684(4) 7_556 ?
O1 Na4 2.749(4) 3_545 ?
O1 K1 2.749(4) 3_545 ?
O2 Mo1 1.758(3) 7_556 ?
O3 Na2 2.468(4) 3 ?
O3 Na3 2.686(3) 2_655 ?
O4 Mo1 1.771(3) 3 ?
O4 Na1 2.195(3) 4 ?
O4 Mg1 2.195(3) 4 ?
O4 Na2 2.393(3) 3 ?
O4 K1 3.093(4) 3 ?
O5 Mo2 1.765(3) 7_565 ?
O5 Na1 2.170(3) 4 ?
O5 Mg1 2.170(3) 4 ?
O5 Na2 2.447(3) 3 ?
O5 K1 3.192(4) 7_566 ?
O6 Mo2 1.781(3) 7_566 ?
O6 Na1 2.203(3) 4 ?
O6 Mg1 2.203(3) 4 ?
O6 Na1 2.292(4) 6_566 ?
O6 Mg1 2.292(4) 6_566 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Mo1 O2 102.2(2) 8_456 7_556 ?
O2 Mo1 O4 109.22(15) 8_456 4_546 ?
O2 Mo1 O4 112.56(14) 7_556 4_546 ?
O2 Mo1 O4 112.56(14) 8_456 3_445 ?
O2 Mo1 O4 109.22(15) 7_556 3_445 ?
O4 Mo1 O4 110.8(2) 4_546 3_445 ?
O2 Mo1 Na3 67.98(13) 8_456 3_445 ?
O2 Mo1 Na3 45.86(11) 7_556 3_445 ?
O4 Mo1 Na3 152.32(10) 4_546 3_445 ?
O4 Mo1 Na3 94.76(10) 3_445 3_445 ?
O2 Mo1 Na3 45.86(11) 8_456 4_546 ?
O2 Mo1 Na3 67.98(13) 7_556 4_546 ?
O4 Mo1 Na3 94.76(10) 4_546 4_546 ?
O4 Mo1 Na3 152.32(10) 3_445 4_546 ?
Na3 Mo1 Na3 62.894(10) 3_445 4_546 ?
O2 Mo1 Na1 133.33(11) 8_456 1_556 ?
O2 Mo1 Na1 85.26(11) 7_556 1_556 ?
O4 Mo1 Na1 31.62(10) 4_546 1_556 ?
O4 Mo1 Na1 107.81(10) 3_445 1_556 ?
Na3 Mo1 Na1 130.93(2) 3_445 1_556 ?
Na3 Mo1 Na1 99.50(2) 4_546 1_556 ?
O2 Mo1 Na1 85.26(11) 8_456 2 ?
O2 Mo1 Na1 133.33(11) 7_556 2 ?
O4 Mo1 Na1 107.81(10) 4_546 2 ?
O4 Mo1 Na1 31.62(10) 3_445 2 ?
Na3 Mo1 Na1 99.50(2) 3_445 2 ?
Na3 Mo1 Na1 130.93(2) 4_546 2 ?
Na1 Mo1 Na1 122.54(5) 1_556 2 ?
O2 Mo1 Na1 29.52(11) 8_456 8_456 ?
O2 Mo1 Na1 126.78(12) 7_556 8_456 ?
O4 Mo1 Na1 107.20(10) 4_546 8_456 ?
O4 Mo1 Na1 87.11(10) 3_445 8_456 ?
Na3 Mo1 Na1 83.72(2) 3_445 8_456 ?
Na3 Mo1 Na1 74.97(2) 4_546 8_456 ?
Na1 Mo1 Na1 138.72(4) 1_556 8_456 ?
Na1 Mo1 Na1 57.06(4) 2 8_456 ?
O2 Mo1 Na1 126.78(12) 8_456 7_556 ?
O2 Mo1 Na1 29.52(12) 7_556 7_556 ?
O4 Mo1 Na1 87.11(10) 4_546 7_556 ?
O4 Mo1 Na1 107.20(10) 3_445 7_556 ?
Na3 Mo1 Na1 74.97(2) 3_445 7_556 ?
Na3 Mo1 Na1 83.72(2) 4_546 7_556 ?
Na1 Mo1 Na1 57.06(4) 1_556 7_556 ?
Na1 Mo1 Na1 138.72(4) 2 7_556 ?
Na1 Mo1 Na1 155.04(5) 8_456 7_556 ?
O2 Mo1 Na2 75.00(12) 8_456 1_556 ?
O2 Mo1 Na2 110.84(12) 7_556 1_556 ?
O4 Mo1 Na2 35.84(10) 4_546 1_556 ?
O4 Mo1 Na2 136.31(10) 3_445 1_556 ?
Na3 Mo1 Na2 125.87(4) 3_445 1_556 ?
Na3 Mo1 Na2 62.98(4) 4_546 1_556 ?
Na1 Mo1 Na2 59.64(3) 1_556 1_556 ?
Na1 Mo1 Na2 115.55(3) 2 1_556 ?
Na1 Mo1 Na2 82.73(2) 8_456 1_556 ?
Na1 Mo1 Na2 99.20(2) 7_556 1_556 ?
O2 Mo1 Na2 110.84(12) 8_456 . ?
O2 Mo1 Na2 75.00(12) 7_556 . ?
O4 Mo1 Na2 136.31(10) 4_546 . ?
O4 Mo1 Na2 35.84(10) 3_445 . ?
Na3 Mo1 Na2 62.98(4) 3_445 . ?
Na3 Mo1 Na2 125.87(4) 4_546 . ?
Na1 Mo1 Na2 115.55(3) 1_556 . ?
Na1 Mo1 Na2 59.64(3) 2 . ?
Na1 Mo1 Na2 99.20(2) 8_456 . ?
Na1 Mo1 Na2 82.73(2) 7_556 . ?
Na2 Mo1 Na2 171.15(8) 1_556 . ?
O3 Mo2 O1 108.81(18) . 8_455 ?
O3 Mo2 O5 111.17(15) . 7_565 ?
O1 Mo2 O5 107.64(16) 8_455 7_565 ?
O3 Mo2 O6 108.16(15) . 7_566 ?
O1 Mo2 O6 109.32(17) 8_455 7_566 ?
O5 Mo2 O6 111.70(15) 7_565 7_566 ?
O3 Mo2 Na1 93.18(11) . 4 ?
O1 Mo2 Na1 143.53(13) 8_455 4 ?
O5 Mo2 Na1 89.96(10) 7_565 4 ?
O6 Mo2 Na1 34.53(11) 7_566 4 ?
O3 Mo2 Na1 86.44(11) . 6_565 ?
O1 Mo2 Na1 104.60(12) 8_455 6_565 ?
O5 Mo2 Na1 28.35(11) 7_565 6_565 ?
O6 Mo2 Na1 135.58(11) 7_566 6_565 ?
Na1 Mo2 Na1 105.49(3) 4 6_565 ?
O3 Mo2 Na4 128.83(11) . 1_554 ?
O1 Mo2 Na4 45.57(13) 8_455 1_554 ?
O5 Mo2 Na4 62.30(11) 7_565 1_554 ?
O6 Mo2 Na4 121.57(11) 7_566 1_554 ?
Na1 Mo2 Na4 134.84(5) 4 1_554 ?
Na1 Mo2 Na4 67.16(3) 6_565 1_554 ?
O3 Mo2 K1 128.83(11) . 1_554 ?
O1 Mo2 K1 45.57(13) 8_455 1_554 ?
O5 Mo2 K1 62.30(11) 7_565 1_554 ?
O6 Mo2 K1 121.57(11) 7_566 1_554 ?
Na1 Mo2 K1 134.84(5) 4 1_554 ?
Na1 Mo2 K1 67.16(3) 6_565 1_554 ?
Na4 Mo2 K1 0 1_554 1_554 ?
O3 Mo2 Na2 37.54(11) . 3 ?
O1 Mo2 Na2 146.07(14) 8_455 3 ?
O5 Mo2 Na2 93.82(11) 7_565 3 ?
O6 Mo2 Na2 85.47(11) 7_566 3 ?
Na1 Mo2 Na2 59.20(4) 4 3 ?
Na1 Mo2 Na2 81.94(2) 6_565 3 ?
Na4 Mo2 Na2 148.252(14) 1_554 3 ?
K1 Mo2 Na2 148.252(14) 1_554 3 ?
O3 Mo2 K1 140.16(11) . 5_566 ?
O1 Mo2 K1 43.21(14) 8_455 5_566 ?
O5 Mo2 K1 105.54(12) 7_565 5_566 ?
O6 Mo2 K1 70.57(11) 7_566 5_566 ?
Na1 Mo2 K1 101.93(5) 4 5_566 ?
Na1 Mo2 K1 123.34(2) 6_565 5_566 ?
Na4 Mo2 K1 58.355(10) 1_554 5_566 ?
K1 Mo2 K1 58.355(10) 1_554 5_566 ?
Na2 Mo2 K1 153.355(19) 3 5_566 ?
O2 Mg1 O5 102.92(14) . 4_545 ?
O2 Mg1 O1 95.54(14) . 8_455 ?
O5 Mg1 O1 87.25(13) 4_545 8_455 ?
O2 Mg1 O4 169.01(13) . 4_545 ?
O5 Mg1 O4 83.44(12) 4_545 4_545 ?
O1 Mg1 O4 93.70(14) 8_455 4_545 ?
O2 Mg1 O6 89.92(14) . 4_545 ?
O5 Mg1 O6 164.64(14) 4_545 4_545 ?
O1 Mg1 O6 100.01(14) 8_455 4_545 ?
O4 Mg1 O6 82.60(12) 4_545 4_545 ?
O2 Mg1 O6 80.63(13) . 6_565 ?
O5 Mg1 O6 90.10(12) 4_545 6_565 ?
O1 Mg1 O6 174.75(14) 8_455 6_565 ?
O4 Mg1 O6 90.50(12) 4_545 6_565 ?
O6 Mg1 O6 83.64(13) 4_545 6_565 ?
O2 Mg1 Na1 83.56(10) . 7 ?
O5 Mg1 Na1 129.44(11) 4_545 7 ?
O1 Mg1 Na1 142.71(12) 8_455 7 ?
O4 Mg1 Na1 85.49(9) 4_545 7 ?
O6 Mg1 Na1 42.84(9) 4_545 7 ?
O6 Mg1 Na1 40.80(8) 6_565 7 ?
O2 Mg1 Mg1 83.56(10) . 7 ?
O5 Mg1 Mg1 129.44(11) 4_545 7 ?
O1 Mg1 Mg1 142.71(12) 8_455 7 ?
O4 Mg1 Mg1 85.49(9) 4_545 7 ?
O6 Mg1 Mg1 42.84(9) 4_545 7 ?
O6 Mg1 Mg1 40.80(8) 6_565 7 ?
Na1 Mg1 Mg1 0.00(5) 7 7 ?
O2 Mg1 Na2 141.15(11) . . ?
O5 Mg1 Na2 43.22(9) 4_545 . ?
O1 Mg1 Na2 99.92(12) 8_455 . ?
O4 Mg1 Na2 41.88(8) 4_545 . ?
O6 Mg1 Na2 121.65(10) 4_545 . ?
O6 Mg1 Na2 81.14(9) 6_565 . ?
Na1 Mg1 Na2 103.87(7) 7 . ?
Mg1 Mg1 Na2 103.87(7) 7 . ?
O2 Mg1 Na4 127.75(11) . 1_554 ?
O5 Mg1 Na4 107.54(10) 4_545 1_554 ?
O1 Mg1 Na4 46.05(11) 8_455 1_554 ?
O4 Mg1 Na4 56.82(9) 4_545 1_554 ?
O6 Mg1 Na4 69.65(9) 4_545 1_554 ?
O6 Mg1 Na4 139.19(10) 6_565 1_554 ?
Na1 Mg1 Na4 106.81(6) 7 1_554 ?
Mg1 Mg1 Na4 106.81(6) 7 1_554 ?
Na2 Mg1 Na4 87.19(4) . 1_554 ?
O2 Mg1 K1 127.75(11) . 1_554 ?
O5 Mg1 K1 107.54(10) 4_545 1_554 ?
O1 Mg1 K1 46.05(11) 8_455 1_554 ?
O4 Mg1 K1 56.82(9) 4_545 1_554 ?
O6 Mg1 K1 69.65(9) 4_545 1_554 ?
O6 Mg1 K1 139.19(10) 6_565 1_554 ?
Na1 Mg1 K1 106.81(6) 7 1_554 ?
Mg1 Mg1 K1 106.81(6) 7 1_554 ?
Na2 Mg1 K1 87.19(4) . 1_554 ?
Na4 Mg1 K1 0.00(8) 1_554 1_554 ?
O2 Mg1 Na4 123.10(10) . 5_566 ?
O5 Mg1 Na4 53.59(9) 4_545 5_566 ?
O1 Mg1 Na4 41.73(11) 8_455 5_566 ?
O4 Mg1 Na4 67.89(9) 4_545 5_566 ?
O6 Mg1 Na4 125.46(10) 4_545 5_566 ?
O6 Mg1 Na4 138.26(10) 6_565 5_566 ?
Na1 Mg1 Na4 153.11(7) 7 5_566 ?
Mg1 Mg1 Na4 153.11(7) 7 5_566 ?
Na2 Mg1 Na4 58.68(5) . 5_566 ?
Na4 Mg1 Na4 55.83(2) 1_554 5_566 ?
K1 Mg1 Na4 55.83(2) 1_554 5_566 ?
O4 Na2 O4 144.57(18) 3_445 4_545 ?
O4 Na2 O5 87.88(11) 3_445 4_545 ?
O4 Na2 O5 73.73(11) 4_545 4_545 ?
O4 Na2 O5 73.73(11) 3_445 3_445 ?
O4 Na2 O5 87.88(11) 4_545 3_445 ?
O5 Na2 O5 117.22(18) 4_545 3_445 ?
O4 Na2 O3 94.23(11) 3_445 3_445 ?
O4 Na2 O3 114.71(11) 4_545 3_445 ?
O5 Na2 O3 156.54(13) 4_545 3_445 ?
O5 Na2 O3 85.66(11) 3_445 3_445 ?
O4 Na2 O3 114.71(11) 3_445 4_545 ?
O4 Na2 O3 94.23(11) 4_545 4_545 ?
O5 Na2 O3 85.66(11) 4_545 4_545 ?
O5 Na2 O3 156.54(13) 3_445 4_545 ?
O3 Na2 O3 72.22(16) 3_445 4_545 ?
O4 Na2 Na1 37.75(8) 3_445 2 ?
O4 Na2 Na1 123.26(10) 4_545 2 ?
O5 Na2 Na1 112.33(10) 4_545 2 ?
O5 Na2 Na1 37.38(8) 3_445 2 ?
O3 Na2 Na1 82.18(8) 3_445 2 ?
O3 Na2 Na1 141.20(10) 4_545 2 ?
O4 Na2 Mg1 37.75(8) 3_445 2 ?
O4 Na2 Mg1 123.26(10) 4_545 2 ?
O5 Na2 Mg1 112.33(10) 4_545 2 ?
O5 Na2 Mg1 37.38(8) 3_445 2 ?
O3 Na2 Mg1 82.18(8) 3_445 2 ?
O3 Na2 Mg1 141.20(10) 4_545 2 ?
Na1 Na2 Mg1 0.00(2) 2 2 ?
O4 Na2 Mg1 123.26(10) 3_445 . ?
O4 Na2 Mg1 37.75(8) 4_545 . ?
O5 Na2 Mg1 37.38(8) 4_545 . ?
O5 Na2 Mg1 112.33(10) 3_445 . ?
O3 Na2 Mg1 141.20(10) 3_445 . ?
O3 Na2 Mg1 82.18(8) 4_545 . ?
Na1 Na2 Mg1 133.08(8) 2 . ?
Mg1 Na2 Mg1 133.08(8) 2 . ?
O4 Na2 Mo1 161.47(10) 3_445 1_554 ?
O4 Na2 Mo1 25.68(7) 4_545 1_554 ?
O5 Na2 Mo1 96.21(8) 4_545 1_554 ?
O5 Na2 Mo1 88.40(7) 3_445 1_554 ?
O3 Na2 Mo1 89.17(8) 3_445 1_554 ?
O3 Na2 Mo1 83.67(8) 4_545 1_554 ?
Na1 Na2 Mo1 125.38(3) 2 1_554 ?
Mg1 Na2 Mo1 125.38(3) 2 1_554 ?
Mg1 Na2 Mo1 58.83(2) . 1_554 ?
O4 Na2 Mo1 25.68(7) 3_445 . ?
O4 Na2 Mo1 161.47(10) 4_545 . ?
O5 Na2 Mo1 88.40(7) 4_545 . ?
O5 Na2 Mo1 96.21(8) 3_445 . ?
O3 Na2 Mo1 83.67(8) 3_445 . ?
O3 Na2 Mo1 89.17(8) 4_545 . ?
Na1 Na2 Mo1 58.83(2) 2 . ?
Mg1 Na2 Mo1 58.83(2) 2 . ?
Mg1 Na2 Mo1 125.38(3) . . ?
Mo1 Na2 Mo1 171.15(8) 1_554 . ?
O3 Na3 O3 180 5_666 . ?
O3 Na3 O2 74.64(11) 5_666 5_666 ?
O3 Na3 O2 105.36(11) . 5_666 ?
O3 Na3 O2 105.36(11) 5_666 . ?
O3 Na3 O2 74.64(11) . . ?
O2 Na3 O2 180.00(10) 5_666 . ?
O3 Na3 O3 67.83(13) 5_666 6_566 ?
O3 Na3 O3 112.17(13) . 6_566 ?
O2 Na3 O3 103.95(11) 5_666 6_566 ?
O2 Na3 O3 76.05(11) . 6_566 ?
O3 Na3 O3 112.17(13) 5_666 2_655 ?
O3 Na3 O3 67.83(13) . 2_655 ?
O2 Na3 O3 76.05(11) 5_666 2_655 ?
O2 Na3 O3 103.95(11) . 2_655 ?
O3 Na3 O3 180.00(12) 6_566 2_655 ?
O3 Na3 Mo1 93.66(7) 5_666 3 ?
O3 Na3 Mo1 86.34(7) . 3 ?
O2 Na3 Mo1 29.73(8) 5_666 3 ?
O2 Na3 Mo1 150.27(8) . 3 ?
O3 Na3 Mo1 90.79(7) 6_566 3 ?
O3 Na3 Mo1 89.21(7) 2_655 3 ?
O3 Na3 Mo1 86.34(7) 5_666 7_556 ?
O3 Na3 Mo1 93.66(7) . 7_556 ?
O2 Na3 Mo1 150.27(8) 5_666 7_556 ?
O2 Na3 Mo1 29.73(8) . 7_556 ?
O3 Na3 Mo1 89.21(7) 6_566 7_556 ?
O3 Na3 Mo1 90.79(7) 2_655 7_556 ?
Mo1 Na3 Mo1 180 3 7_556 ?
O3 Na3 Na3 48.49(7) 5_666 2_656 ?
O3 Na3 Na3 131.51(7) . 2_656 ?
O2 Na3 Na3 60.58(9) 5_666 2_656 ?
O2 Na3 Na3 119.42(9) . 2_656 ?
O3 Na3 Na3 44.70(7) 6_566 2_656 ?
O3 Na3 Na3 135.30(7) 2_655 2_656 ?
Mo1 Na3 Na3 58.553(5) 3 2_656 ?
Mo1 Na3 Na3 121.447(5) 7_556 2_656 ?
O3 Na3 Na3 131.51(7) 5_666 2_655 ?
O3 Na3 Na3 48.49(7) . 2_655 ?
O2 Na3 Na3 119.42(9) 5_666 2_655 ?
O2 Na3 Na3 60.58(9) . 2_655 ?
O3 Na3 Na3 135.30(7) 6_566 2_655 ?
O3 Na3 Na3 44.70(7) 2_655 2_655 ?
Mo1 Na3 Na3 121.447(5) 3 2_655 ?
Mo1 Na3 Na3 58.553(5) 7_556 2_655 ?
Na3 Na3 Na3 180 2_656 2_655 ?
O3 Na3 Na2 137.93(7) 5_666 3 ?
O3 Na3 Na2 42.07(7) . 3 ?
O2 Na3 Na2 67.24(8) 5_666 3 ?
O2 Na3 Na2 112.76(8) . 3 ?
O3 Na3 Na2 137.76(7) 6_566 3 ?
O3 Na3 Na2 42.24(7) 2_655 3 ?
Mo1 Na3 Na2 60.638(19) 3 3 ?
Mo1 Na3 Na2 119.362(19) 7_556 3 ?
Na3 Na3 Na2 119.191(18) 2_656 3 ?
Na3 Na3 Na2 60.809(18) 2_655 3 ?
O3 Na3 Na2 42.07(7) 5_666 7_556 ?
O3 Na3 Na2 137.93(7) . 7_556 ?
O2 Na3 Na2 112.76(8) 5_666 7_556 ?
O2 Na3 Na2 67.24(8) . 7_556 ?
O3 Na3 Na2 42.24(7) 6_566 7_556 ?
O3 Na3 Na2 137.76(7) 2_655 7_556 ?
Mo1 Na3 Na2 119.362(19) 3 7_556 ?
Mo1 Na3 Na2 60.638(19) 7_556 7_556 ?
Na3 Na3 Na2 60.809(18) 2_656 7_556 ?
Na3 Na3 Na2 119.191(18) 2_655 7_556 ?
Na2 Na3 Na2 180.00(4) 3 7_556 ?
O1 Na4 O1 178.0(2) 8_456 7_556 ?
O1 Na4 O1 97.33(11) 8_456 4_556 ?
O1 Na4 O1 82.53(11) 7_556 4_556 ?
O1 Na4 O1 82.53(11) 8_456 3_455 ?
O1 Na4 O1 97.33(11) 7_556 3_455 ?
O1 Na4 O1 172.3(2) 4_556 3_455 ?
O1 Na4 K1 49.44(9) 8_456 5_567 ?
O1 Na4 K1 130.39(8) 7_556 5_567 ?
O1 Na4 K1 47.89(8) 4_556 5_567 ?
O1 Na4 K1 131.45(8) 3_455 5_567 ?
O1 Na4 Na4 49.44(9) 8_456 5_567 ?
O1 Na4 Na4 130.39(8) 7_556 5_567 ?
O1 Na4 Na4 47.89(8) 4_556 5_567 ?
O1 Na4 Na4 131.45(8) 3_455 5_567 ?
K1 Na4 Na4 0.00(10) 5_567 5_567 ?
O1 Na4 K1 130.39(8) 8_456 5_566 ?
O1 Na4 K1 49.44(9) 7_556 5_566 ?
O1 Na4 K1 131.45(8) 4_556 5_566 ?
O1 Na4 K1 47.89(8) 3_455 5_566 ?
K1 Na4 K1 172.60(19) 5_567 5_566 ?
Na4 Na4 K1 172.60(19) 5_567 5_566 ?
O1 Na4 Na4 130.39(8) 8_456 5_566 ?
O1 Na4 Na4 49.44(9) 7_556 5_566 ?
O1 Na4 Na4 131.45(8) 4_556 5_566 ?
O1 Na4 Na4 47.89(8) 3_455 5_566 ?
K1 Na4 Na4 172.60(19) 5_567 5_566 ?
Na4 Na4 Na4 172.60(19) 5_567 5_566 ?
K1 Na4 Na4 0.00(10) 5_566 5_566 ?
O1 Na4 Mo2 27.90(7) 8_456 1_556 ?
O1 Na4 Mo2 150.24(13) 7_556 1_556 ?
O1 Na4 Mo2 105.57(8) 4_556 1_556 ?
O1 Na4 Mo2 70.85(8) 3_455 1_556 ?
K1 Na4 Mo2 62.91(4) 5_567 1_556 ?
Na4 Na4 Mo2 62.91(4) 5_567 1_556 ?
K1 Na4 Mo2 113.45(6) 5_566 1_556 ?
Na4 Na4 Mo2 113.45(6) 5_566 1_556 ?
O1 Na4 Mo2 150.24(13) 8_456 2 ?
O1 Na4 Mo2 27.90(7) 7_556 2 ?
O1 Na4 Mo2 70.85(8) 4_556 2 ?
O1 Na4 Mo2 105.57(8) 3_455 2 ?
K1 Na4 Mo2 113.45(6) 5_567 2 ?
Na4 Na4 Mo2 113.45(6) 5_567 2 ?
K1 Na4 Mo2 62.91(4) 5_566 2 ?
Na4 Na4 Mo2 62.91(4) 5_566 2 ?
Mo2 Na4 Mo2 127.24(9) 1_556 2 ?
O1 Na4 Na2 88.99(10) 8_456 5_566 ?
O1 Na4 Na2 88.99(10) 7_556 5_566 ?
O1 Na4 Na2 86.15(10) 4_556 5_566 ?
O1 Na4 Na2 86.15(10) 3_455 5_566 ?
K1 Na4 Na2 86.30(10) 5_567 5_566 ?
Na4 Na4 Na2 86.30(10) 5_567 5_566 ?
K1 Na4 Na2 86.30(10) 5_566 5_566 ?
Na4 Na4 Na2 86.30(10) 5_566 5_566 ?
Mo2 Na4 Na2 63.62(4) 1_556 5_566 ?
Mo2 Na4 Na2 63.62(4) 2 5_566 ?
O1 Na4 Na1 146.33(13) 8_456 2 ?
O1 Na4 Na1 35.65(9) 7_556 2 ?
O1 Na4 Na1 79.30(8) 4_556 2 ?
O1 Na4 Na1 105.09(9) 3_455 2 ?
K1 Na4 Na1 118.70(7) 5_567 2 ?
Na4 Na4 Na1 118.70(7) 5_567 2 ?
K1 Na4 Na1 65.90(5) 5_566 2 ?
Na4 Na4 Na1 65.90(5) 5_566 2 ?
Mo2 Na4 Na1 171.86(8) 1_556 2 ?
Mo2 Na4 Na1 60.29(2) 2 2 ?
Na2 Na4 Na1 123.79(5) 5_566 2 ?
Mo2 O1 Na1 137.1(2) 8_556 8_556 ?
Mo2 O1 Mg1 137.1(2) 8_556 8_556 ?
Na1 O1 Mg1 0.000(18) 8_556 8_556 ?
Mo2 O1 K1 106.53(17) 8_556 7_556 ?
Na1 O1 K1 98.31(15) 8_556 7_556 ?
Mg1 O1 K1 98.31(15) 8_556 7_556 ?
Mo2 O1 Na4 106.53(17) 8_556 7_556 ?
Na1 O1 Na4 98.31(15) 8_556 7_556 ?
Mg1 O1 Na4 98.31(15) 8_556 7_556 ?
K1 O1 Na4 0 7_556 7_556 ?
Mo2 O1 Na4 110.80(19) 8_556 3_545 ?
Na1 O1 Na4 106.53(15) 8_556 3_545 ?
Mg1 O1 Na4 106.53(15) 8_556 3_545 ?
K1 O1 Na4 82.67(11) 7_556 3_545 ?
Na4 O1 Na4 82.67(11) 7_556 3_545 ?
Mo2 O1 K1 110.80(19) 8_556 3_545 ?
Na1 O1 K1 106.53(15) 8_556 3_545 ?
Mg1 O1 K1 106.53(15) 8_556 3_545 ?
K1 O1 K1 82.67(11) 7_556 3_545 ?
Na4 O1 K1 82.67(11) 7_556 3_545 ?
Na4 O1 K1 0.00(13) 3_545 3_545 ?
Mo1 O2 Mg1 126.94(18) 7_556 . ?
Mo1 O2 Na3 104.41(16) 7_556 . ?
Mg1 O2 Na3 127.55(15) . . ?
Mo2 O3 Na2 116.94(15) . 3 ?
Mo2 O3 Na3 121.78(16) . . ?
Na2 O3 Na3 94.71(11) 3 . ?
Mo2 O3 Na3 135.46(17) . 2_655 ?
Na2 O3 Na3 90.75(11) 3 2_655 ?
Na3 O3 Na3 86.82(9) . 2_655 ?
Mo1 O4 Na1 123.36(16) 3 4 ?
Mo1 O4 Mg1 123.36(16) 3 4 ?
Na1 O4 Mg1 0.00(4) 4 4 ?
Mo1 O4 Na2 118.48(16) 3 3 ?
Na1 O4 Na2 100.37(12) 4 3 ?
Mg1 O4 Na2 100.37(12) 4 3 ?
Mo1 O4 K1 96.46(12) 3 3 ?
Na1 O4 K1 86.75(10) 4 3 ?
Mg1 O4 K1 86.75(10) 4 3 ?
Na2 O4 K1 129.81(13) 3 3 ?
Mo2 O5 Na1 128.93(17) 7_565 4 ?
Mo2 O5 Mg1 128.93(17) 7_565 4 ?
Na1 O5 Mg1 0.00(6) 4 4 ?
Mo2 O5 Na2 131.02(17) 7_565 3 ?
Na1 O5 Na2 99.40(12) 4 3 ?
Mg1 O5 Na2 99.40(12) 4 3 ?
Mo2 O5 K1 88.39(12) 7_565 7_566 ?
Na1 O5 K1 93.24(11) 4 7_566 ?
Mg1 O5 K1 93.24(11) 4 7_566 ?
Na2 O5 K1 80.50(11) 3 7_566 ?
Mo2 O6 Na1 140.61(19) 7_566 4 ?
Mo2 O6 Mg1 140.61(19) 7_566 4 ?
Na1 O6 Mg1 0.000(9) 4 4 ?
Mo2 O6 Na1 119.34(16) 7_566 6_566 ?
Na1 O6 Na1 96.36(13) 4 6_566 ?
Mg1 O6 Na1 96.36(13) 4 6_566 ?
Mo2 O6 Mg1 119.34(16) 7_566 6_566 ?
Na1 O6 Mg1 96.36(13) 4 6_566 ?
Mg1 O6 Mg1 96.36(13) 4 6_566 ?
Na1 O6 Mg1 0.00(7) 6_566 6_566 ?

